AN INVESTIGATION OF NANOTUBE-INTEGRATED…

Figure 6 Atomic model of a single (crossed) layer of buckysheets For the buckysheet atomic simulation model, two (10, 10) single-walled CNTs formed a “separated cross” in a unit cell. The separation distance between the two crossed nanotubes was initially determined by minimizing the strain energy of the model. Under the periodic boundary conditions, the unit cell was replicated in all three dimensions. We also carried out atomic simulation of the multilayer buckysheets, where several single layer buckysheets were modeled in one unit cell and the periodic boundary conditions were applied. The separation distance among the layers was optimized in the same way as mentioned above. The molecular mechanics/dynamics simulations calculations were performed using Cerius2/Accelrys software [9]. The application of strain was performed by uniformly expanding the dimensions of the MD cell in the direction of the deformation, then re-scaling the new coordinates of the atoms to fit within the new dimensions [10]. After the initial deformation, the MD simulation was continued and the atoms were allowed to equilibrate within the new MD cell dimensions. In the following increments of deformation, this process was repeated. In each increment, the strain energy was minimized and recorded, then the Young’s modulus could be calculated from the second derivative of the strain energy density with respect to various strains [11-13]:

ij

1 E ( )S V ij

(7)

where V is the volume of the solid, E is the total internal energy,

ij

is the strain tensor, and the subscript S denotes constant

entropy.

V.

MOLECULAR DYNAMIC SIMULATION RESULTS AND REMARKS

For the single-walled CNT (10,10), the simulation results show that the Young’s modulus ranges from 0.75 TPa to 0.9 TPa, which is lower than the value 0.972 TPa obtained by [10], and higher than the results (0.5~ 0.6 TPa) from [12,13]. In the simulation of the single layer buckypaper, the separation distance between the crossed CNTs in the radius direction of the model is 3.1 nm. The Young’s Modulus of 0.3 TPa for the buckypaper was obtained. When increase the separation distance from 2nm to 7nm between nanotubes in the buckypaper model, the value of Young’s modulus reduced from 0.349 TPa to 0.267 TPa, as shown in Figure 7. 0.35 0.34

Youngs Modulus, TPa

0.33 0.32 0.31 0.3 0.29 0.28 0.27 0.26

2

2.5

3

3.5 4 4.5 5 5.5 Distance between nanotubes, A

6

6.5

7

Fig. 7 Young’s modulus decreases when increase the separation distance in single layer buckysheets As to the multilayer buckysheet, the simulation results are depicted in Figure 8. The Young’s modulus decreases from 0.326TPa to 0.189 TPa while the layer number of the buckysheet varies from 1 to 5, which is due to the gap between ISSN: 2278-7461

www.ijeijournal.com

P a g e | 35

Advertisement